l13 14 fracture
Post on 17-Oct-2015
Embed Size (px)
If cannot bear such conditions1
FailureDuctile and brittle fractureFracture toughnessFundamentals of fracture mechanics
An oil tanker that fractured in a brittle manner by crack propagation around its girth. (Photography by Neal Boenzi. Reprinted with permission from The New York Times.)
Failure in structures leads to lost ofproperties and sometimes lost ofhuman lives.2Types of fracture
Fracture is the separation of a body into two or more pieces in response to an imposed stress that is static and at temperatures that are low relative to the melting temperature of the material.3Failure modes
Moderately ductile fracture after somenecking.Brittle fracture without anyplastic deformation.Highly ductile fracture inwhich the specimen necks down to a point4Ductile fracture is almost always preferred to brittle one.Ductile fracture
Highly ductile fracture inwhich the specimen necks down to a point
Cup-and-cone fracture in aluminum.
Final shear fracture.Initial necking. Small cavity formationCoalescence ofcavities to form a crackCrackpropagation6Tough ductile fractureDuctile fracture is a much less seriousproblem in engineering materials sincefailure can be detected beforehand dueto observable plastic deformationprior to failure.
Under uniaxial tensile force, afternecking, microvoids form andcoalesce to form crack, which thenpropagate in the direction normal tothe tensile axis.
The crack then rapidly propagatethrough the periphery along the shearplane, leaving the cub andcone fracture.7Microvoid formation, growth andcoalescence
Microvoids are easily formed at inclusions, intermetallic or second-phase particles and grain boundaries. Growth and coalescence of microvoids progress as the local applied load increases.
Random planar arrayof particles acting asvoid initiatorsGrowth of voids to joineach other as the appliedstress increases.Linkage or coalescenceof these voids to form free fracture surface.8Ductile fracture of alloys9
If materials is stretched, it firstly deforms uniformly. Inclusions stress concentratorsFormation of microvoids from secondphase particles
1) Decohesion at particle -matrix interface.2) Fracture of brittle particle3) Decohesion of an interface associated with shear deformation or grainboundary sliding.
Decohesion of carbide particlesfrom Ti matrix.Fractured carbides aidingmicrovoid formation.10Brittle fracture
Scanning electronfractograph of ductilecast iron showing a transgranular fracture surface.Scanning electronfractograph showingan intergranularfracture surface.12
Nature of fracture: brittleCharacteristic for ceramics and glasses
Distinct characteristics of brittle fracture surfaces:
1) The absence of gross plastic deformation.2) Grainy or Faceted texture.3) River marking or stress lines.13Intergranular fracture Intergranular failure isa moderate to low energybrittle fracture mode resultingfrom grain boundaryseparation or segregation ofembrittling particles orprecipitates.
Embrittling grainboundary particles areweakly bonded with thematrix, high free energyand unstable, which leads topreferential crackpropagation path.
Intergranular fracture with and withoutmicrovoid coalescence14Strength and toughness15
StrengthResistance of a materialto plastic flowToughnessResistance of a materialto the propagationof a crackHow concerned should you be if you read in the paper that cracks have been detected in the pressure vessel of the nuclear reactor of the power station a few miles away?Testing for toughness
This type of test provides a comparison of the toughness of materials
however, it does not provide a way to express toughness as a material property (no true material property that is independent on size and shape of the test sample)Tear testImpact testMeasuring the energy 16Introduction to fracture mechanicsThe fracture strength of a solid material is a function of the cohesive forces that exist between atoms.On this basis, the theoretical cohesive strength of a brittle elastic solid has been estimated to be approximately E/10, where E is the modulusof elasticity.The experimental fracture strengths of most engineering materialsnormally lie between 10 and 1000 times below this theoretical value. Why?
surface energyunstrained interatomic spacing17Stress concentration
Crack reduces the cross section => increase in stressWhat will happen with tough material?Cracks concentrate stressFlaws are detriment to the fracture strength because an applied stress may be amplified or concentrated at the tip, the magnitude of this amplification depends on crack orientation and geometry. 18What force is required to break the samples?
19Theories of brittle fracture
Schematic stress profile along the line XXthe magnitude of this localized stressdiminishes with distance away from the crack tip
The maximum stress at the crack tip
stress concentration factorA measure of the degree to which an external stress is amplified at the tip of a crack21Problem221. Consider a circular hole in a plate loaded in tension. When will material near the hole yield?
2. A plate with a rectangular section 500 mm by 15 mm carries a tensile load of 50kN. It is made of a ductile metal with a yield strength of 50 MPa. The plate contains an elliptical hole of length 100 mm and a minimum radius of 1 mm, oriented as shown in the diagram. What is
(a) the nominal stress(b) The maximum stress in the plate?(c) Will the plate start to yield? (d) Will it collapse completely?Theoretical stress concentration factorcurves
Griffith theory of brittle fractureInherent defects in brittlematerials lead to stressconcentration.
If stress exceeds the cohesive strength of bonds, crack extension is possible.Thermodynamic criterion: There are two energies to be taken into account when a crack propagates:New surfaces should be created and a certain amount of energy must be provided to create them;Elastic strain energy stored in the stressed material is released during crack propagation.
Theory of brittle fracture25
The stress required tocreate the new crack surfaceCritical stress for crack propagationThe strain energy release rate (G) is higher for higher loads and larger cracks. If the strain energy released exceeds a critical value, then the crack will grow spontaneously. For brittle materials, stress can be equal to the surface energy of the (two) new crack surfaces; in other words, in brittle materials, a crack will grow spontaneously if the strain energy released is equal to or greater than the energy required to grow the crack surface(s).
The stability condition can be written as
elastic energy released (G) = surface energy created (2)
If the elastic energy release is less than the critical value, the crack will not grow.G 2 ProblemA relatively large plate of a glass is subjected to a tensile stress of 40 MPa. If the specific surface energy and modulus of elasticity for this glass are 0.3 J/m2 and 69 GPa, respectively, determine the maximum length of a surface flaw that is possible without fracture.
26Problem: Properties of SiAlON Ceramics27Assume that an advanced ceramic, SiAlON (silicon aluminum oxynitride),has a tensile strength of 414 MPa. Let us assume that this value is for a flaw-free ceramic. (In practice, it is almost impossible to produce flaw-free ceramics.)A crack 0.025 cm deep is observed before a SiAlON part is tested.The part unexpectedly fails at a stress of 3.5 MPa by propagation of the crack. Estimate the radius of the crack tip.
basic modes of crack tip deformation
KIC the critical stress intensity in mode I fracture (plain strain)
critical stress for crack propagation
28K = (EG) 1/2
Fracture toughnessFT is a material property;Value is independent of the way it is measured;Can be used for designFracture toughness of a material is obtained by determiningthe ability of a material to withstand the load in the presence ofa sharp crack before failure.
Y is a dimensionless parameter or function that depends on both crack and specimen sizes and geometries, as well as the manner of load application29Crack propagates when the stress intensity factor exceeds a critical value. Energy release rateIrwin later modified the Griffith theory by replacing the term 2 with the potential strain energy release rate GWhen a samples fractures, a new surface is created => necessary conditions for fracture sufficient energy releaseG 2The critical condition to which the crackpropagates to cause global failure is when this G value exceeds the critical value
Irwin showed that G is measurable and can be related to the stress intensity factor, K
30Y values of various crack geometries
A plastic zone forms at the crack tip where the stress would otherwise exceed the yield strength
Size of process zone:32Brittle cleavage fracture
Materials of high yield strength
Near tip stress are very high => tear the atomic bonds apart => increase in the crack length results in increase in K, causing crack to accelerate
33Fracture toughness and designIf the KIC value of material is known and the presence of a crack is allowed, we can then monitor the crack propagation during service prior to failure => How long we can use the component before it fails.
Brittle materials, for which appreciable plastic deformation is not possible in front of an advancing crack, have low KIc values and are vulnerable to catastrophic failure.34